Synthesis and structural study of the partially disordered complex hexagonal phase δ<sub>1</sub>-MnZn<sub>9.7</sub>.
Mondal, Amit; Pan, Rahul; Kuila, Sandip Kumar; Dey, Riju; Jana, Partha Pratim; Acta crystallographica Section B, Structural science, crystal engineering and materials 80 (2024) 688–694; doi:10.1107/S2052520624008096

data_2023290
_publ_section_title
;
 Synthesis and structural study of the partially disordered complex
 hexagonal phase &#x3b4;<sub>1</sub>-MnZn<sub>9.7</sub>.
;
_journal_coeditor_code           DK5133SUP1
_journal_issue                   6
_journal_name_full
'Acta crystallographica Section B, Structural science, crystal engineering and materials'
_journal_page_first              688
_journal_page_last               694
_journal_paper_doi               10.1107/S2052520624008096
_journal_volume                  80
_journal_year                    2024
_chemical_formula_sum            'Mn13 Zn126.103'
_chemical_formula_weight         8958.8
_space_group_IT_number           194
_space_group_name_Hall           '-P 6c 2c'
_space_group_name_H-M_alt        'P 63/m m c'
_symmetry_cell_setting           hexagonal
_symmetry_Int_Tables_number      194
_symmetry_space_group_name_Hall  '-P 6c 2c'
_symmetry_space_group_name_H-M   'P 63/m m c'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            4
_cell_length_a                   12.9085(2)
_cell_length_b                   12.9085(2)
_cell_length_c                   57.6528(10)
_cell_measurement_reflns_used    8471
_cell_measurement_temperature    293
_cell_measurement_theta_max      30.47
_cell_measurement_theta_min      3.16
_cell_volume                     8319.6(2)
_diffrn_ambient_temperature      293
_diffrn_measured_fraction_theta_full 0.98
_diffrn_measured_fraction_theta_max 0.96
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Bruker Photon II'
_diffrn_measurement_method       'Bruker Photon II'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'X-ray tube'
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0717
_diffrn_reflns_av_unetI/netI     0.0332
_diffrn_reflns_limit_h_max       18
_diffrn_reflns_limit_h_min       -17
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -18
_diffrn_reflns_limit_l_max       73
_diffrn_reflns_limit_l_min       -72
_diffrn_reflns_number            47922
_diffrn_reflns_theta_full        28.61
_diffrn_reflns_theta_max         30.53
_diffrn_reflns_theta_min         1.86
_exptl_absorpt_coefficient_mu    37.416
_exptl_absorpt_correction_T_max  0.7461
_exptl_absorpt_correction_T_min  0.3565
_exptl_absorpt_correction_type   multi-scan
_exptl_crystal_colour            silvery
_exptl_crystal_density_diffrn    7.1525
_exptl_crystal_description       bar-shaped
_exptl_crystal_F_000             16432
_exptl_crystal_size_max          0.06
_exptl_crystal_size_mid          0.03
_exptl_crystal_size_min          0.02
_refine_diff_density_max         2.24
_refine_diff_density_min         -2.61
_refine_ls_extinction_coef       930(80)
_refine_ls_extinction_method
'B-C type 1 Gaussian isotropic (Becker & Coppens, 1974)'
_refine_ls_goodness_of_fit_gt    1.19
_refine_ls_goodness_of_fit_ref   1.15
_refine_ls_number_constraints    0
_refine_ls_number_parameters     317
_refine_ls_number_reflns         4638
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0475
_refine_ls_R_factor_gt           0.0262
_refine_ls_shift/su_max          0.0378
_refine_ls_shift/su_mean         0.0038
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     w=1/(\s^2^(I)+0.0004I^2^)
_refine_ls_weighting_scheme      sigma
_refine_ls_wR_factor_gt          0.0529
_refine_ls_wR_factor_ref         0.0604
_reflns_number_gt                3405
_reflns_number_total             4638
_reflns_threshold_expression     I>3\s(I)
_publcif_datablock.id            {5f7e8d18-1695-4a6d-8d90-48477f403477}
_publcif_info_exptl_table_max_cols 4
_publcif_info_exptl_table_use_headnotes n
_cod_data_source_file            dk5133sup1.cif
_cod_data_source_block           crystal2
_cod_depositor_comments
'Adding full bibliography for 2023289--2023290.cif.'
_cod_original_sg_symbol_Hall     '-P 6c;-2c'
_cod_database_code               2023290
_cod_database_fobs_code          2023290
_publcif_funding_html
;
;